Fully coupled thermomechanical finite element ... - Clemson University

Q1

**Fully** **coupled** **thermomechanical** **finite** **element**

analysis of material evolution during

friction-stir welding of AA5083

M Grujicic 1 *, T He 1 , G Arakere 1 , H V Yalavarthy 1 , C-F Yen 2 , and B A Cheeseman 2

1 Department of Mechanical Engineering, **Clemson** **University**, **Clemson**, South Carolina, USA

2 Army Research Laboratory, Aberdeen, Proving Ground, Maryland, USA

The manuscript was received on 28 July 2009 and was accepted after revision for publication on 3 September 2009.

DOI: 10.1243/09544054JEM1750

Abstract: Interactions between the rotating and advancing pin-shaped tool (terminated at one

end with a circular–cylindrical shoulder) with the clamped welding plates and the associated

material and heat transport during a friction-stir welding (FSW) process are studied computationally

using a fully **coupled** **thermomechanical** **finite** **element** analysis. To surmount potential

numerical problems associated with extensive mesh distortions/entanglement, an arbitrary

Lagrangian–Eulerian (ALE) formulation was used, which enabled adaptive remeshing (to

ensure the continuing presence of a high-quality mesh) while allowing full tracking of the

material-free surfaces. To demonstrate the utility of the present computational approach, the

analysis is applied to the case of FSW of AA5083 (a solid–solution strengthened and strainhardened/stabilized

Al–Mg wrought alloy). To account for the competition between plastic

deformation-controlled strengthening and dynamic recrystallization-induced softening phenomena

during the FSW process, the original Johnson–Cook strain and strain-rate hardening

and temperature-softening material strength model is modified using the available recrystallization

kinetics experimental data. Lastly, the computational results obtained in the present

work are compared with their experimental counterparts available in the open literature. This

comparison revealed that general trends regarding spatial distribution and temporal evolutions

of various material-state quantities and their dependence on the FSW process parameters are

reasonably well predicted by the present computational approach.

Keywords: fully **coupled** **thermomechanical** **finite** **element** analysis, friction-stir welding,

welding plates, Lagrangian–Eulerian formulation

1 INTRODUCTION

Friction-stir welding (FSW) is a solid-state material

that is generally employed in applications in which the

original material microstructure/properties must

remain unchanged as much as possible after joining

[1–3]. In this process, as shown in Fig. 1(a), a rotating

tool moves along the contacting surfaces of two rigidly

butt-clamped plates. As seen in this figure, the tool

consists of a cylindrical pin that is threaded, at one

end, and equipped with a shoulder, at the other. Also,

during joining, the workpiece (i.e. the two clamped

*Corresponding author: Department of Mechanical Engineering,

**Clemson** **University**, 241 EIB, **Clemson**, SC 29634, USA.

email: mica@ces.clemson.edu

plates) is generally placed on a rigid backing support.

At the same time, the shoulder is forced to make a firm

contact with the top surface of the workpiece. As the

tool (rotates and) moves along the butting surfaces,

heat is being generated at the shoulder/workpiece and,

to a lesser extent, at the pin/workpiece contact surfaces,

as a result of the frictional energy dissipation.

This, in turn, causes an increase in temperature and

gives rise to softening of the material adjacent to these

contacting surfaces. As the tool advances along the

butting surfaces, thermally softened material in front

of the tool is (heavily) deformed, transferred (i.e.

extruded around the tool) to the region behind the tool

and compacted/forged to form a joint/weld. It should

be recognized that FSW can be used not only for butt

joining but also for lap as well as T joints.

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

1

2 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

Fig. 1 (a) A schematic of the friction stir welding (FSW)

process and (b) the main microstructural zones

associated with the typical FSW joint

Since its discovery in 1991 [1], FSW has established

itself as a preferred joining technique for aluminium

components and its applications for joining other

difficult-to-weld metals is gradually expanding. Currently,

this joining process is being widely used in

many industrial sectors such as shipbuilding and

marine, aerospace, railway, land transportation, etc.

In comparison to the traditional fusion welding

technologies, FSW offers a number of advantages,

such as: (a) good mechanical properties in the aswelded

condition; (b) improved safety due to the

absence of toxic fumes or the spatter of molten

material; (c) no requirement for consumables such as

a filler metal or gas shield; (d) ease of process automation;

(e) ability to operate in all positions (horizontal,

vertical, overhead, orbital, etc.), as there is

no weld pool; (f) minimal thickness under/overmatching,

which reduces the need for expensive

post-weld machining; and (g) low environmental

impact. However, some disadvantages of the FSW

process have also been identified, such as: (a) an exit

hole is left after the tool is withdrawn from the

workpiece; (b) relatively large tool press-down and

plate-clamping forces are required; (c) lower flexibility

of the process with respect to variable-thickness

and non-linear welds; and (d) often associated

with lower welding rates than conventional fusionwelding

techniques, although this shortcoming is

somewhat lessened since fewer welding passes are

required.

When analysing the FSW process, a distinction is

often made between the so-called advancing side of

the weld (the side on which the peripheral velocity of

the rotating tool coincides with the transverse velocity

of the tool) and the retreating side (the side on

which the two velocities are aligned in the opposite

directions). It is generally recognized that the differences

in the two weld sides give rise to asymmetry in

heat transfer, material flow, and weld microstructure

properties [4].

FSW normally involves complex interactions and

competition between various **thermomechanical**

processes such as friction–energy dissipation, plastic

deformation and the associated heat dissipation,

material transport/flow, dynamic recrystallization,

local cooling, etc. [5–8]. Metallographic examinations

of the FSW joints typically reveal the existence of the

following four zones (Fig. 1(b)): (a) an uneffected

zone, which is far enough from the weld so that

material microstructure/properties are not altered by

the joining process; (b) the heat affected zone (HAZ)

in which material microstructure/properties are

affected only by the thermal effects associated with

FSW; while this zone is normally found in the case of

fusion welds, the nature of the microstructural

changes may be different in the FSW case due to

generally lower temperatures and a more diffuse heat

source; (c) the **thermomechanical**ly affected zone

(TMAZ), which is located closer than the HAZ zone to

the butting surfaces; consequently both the thermal

and the mechanical aspects of the FSW affect the

material microstructure/properties in this zone and,

typically, the original grains are retained in this zone

although they may have undergone severe plastic

deformation; and (d) the weld nugget, which is the

innermost zone of an FSW joint. As a result of the way

the material is transported from the regions ahead of

the tool to the wake regions behind the tool, this zone

typically contains the so-called onion ring features.

The material in this region has been subjected to the

most severe conditions of plastic deformation and

high-temperature exposure and consequently contains

a very fine dynamically recrystallized (equiaxed

grain) microstructure.

A unique feature of the FSW process is that heat

transfer does not only take place via thermal conduction

but also via transport of the workpiece

material adjacent to the tool from the region in front

to the region behind the advancing tool. In general

both the heat and the mass transfers depend on the

workpiece material properties, tool geometry, and

the FSW process parameters. As mentioned earlier,

mass transport is accompanied by extensive plastic

deformation and dynamic recrystallization of the

transported material. The attendant strain rates as

high as 10/s have been assessed/measured [13, 14].

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

Q2

Q3

The main FSW process parameters that affect both

the weld quality and the process efficiency are: (a)

rotational and transverse velocities of the tool; (b)

tool plunge depth; (c) tool tilt angle; and (d) tool

design/material. Since, in general, higher temperatures

are encountered in the case of higher rotational

and lower transverse tool velocities, it is critical that a

delicate balance between these two velocities is

attained: i.e. when the temperatures are not high

enough and the material has not been sufficiently

softened, the weld zone may develop various flaws/

defects arising from low ductility of the material.

Conversely, when the temperatures are too high

undesirable changes in the material microstructure/

properties may take place and possibly incipient

melting flaws may be created during joining. To

ensure that the necessary level of shoulder/workpiece

contact pressure is attained and that the tool

fully penetrates the weld, the tool plunge depth

(defined as the depth of the lowest point of the

shoulder below the surface of the welded plate) has

to be set correctly. Typically, insufficient tool plunge

depths result in low-quality welds (due to inadequate

forging of the material at the rear of the tool), while

excessive tool plunge depths lead to undermatching

of the weld thickness compared to the base material

thickness. Tool rearward tilting by 2–4 degrees has

been often found to be beneficial since it enhances

the effect of the forging process.

Over the last two decades, considerable experimental

research efforts have been invested towards

providing a better understanding of the FSW joining

mechanism and the accompanying evolution of the

welded material’s microstructure/properties (see, for

example, references [15] to[18]) as well as to rationalizing

the effect of various FSW process parameters

on the weld quality/integrity (e.g. references [19] to

[23]). It should be recognized, however, that the

aforementioned experimental efforts were able to

only correlate the postmortem welded material’s

properties/microstructure with the FSW process

parameters and provided relatively little real-time

insight into the physics of heat/mass transfer and

microstructure evolution processes. It is hoped that

this insight can be gained by carrying out detailed

physically based computational investigations of the

FSW process. An example of such an investigation is

provided in the present manuscript.

A review of the public domain literature revealed

a number of prior research efforts dealing with

numerical investigations of the FSW process.

For example, in a series of papers, Zhang and

co-workers carried out a fairly comprehensive

semi-**coupled** **thermomechanical** **finite** **element**

investigation of the FSW process and the associated

microstructural changes [29–31] . Similarly,

a number of computational solid mechanics and

Thermomechanical **finite** **element** analysis of material evolution 3

computational fluid dynamics investigations were

reported in the literature whose main objective was

to investigate the effect of various FSW process

parameters (including tool design) on the heat/

mass transport processes (e.g. references [29] to

[33]).

The main objective of the present work is to carry

out a detailed **finite** **element** computational investigation

of the effect of various FSW process parameters

on the heat and mass transport of the material

and on the microstructure evolution for the case of

the AA5083 wrought aluminium alloy. While similar

investigations have been carried out by other

researchers (e.g. references [29] to[31]), an effort is

made in the present work to more accurately account

for the competition between strain hardening and

dynamic recrystallization processes in this alloy

during FSW. In other words, while previous investigations

recognized correctly the effect of plastic

strain, strain rate, and temperature on the material

strength, only reversible effects of the temperature

were accounted for. This shortcoming was rectified in

the present work by recognizing that, via dynamic

recrystallization, exposure of the material to high

temperatures may result in permanent microstructure/property

changes.

The organization of the paper is as follows. In various

subsections of section 2, details are provided

regarding the basic formulation of the problem, fully

**coupled** **thermomechanical** **finite** **element** analysis

and its integration, workpiece material models, the

tool/workpiece contact algorithm, and the arbitrary

Lagrangian–Eulerian adaptive meshing method. The

main results obtained in the present work are presented

and discussed in section 3, while the key

conclusions resulting from the present study are

summarized in section 4.

2 COMPUTATIONAL PROCEDURE

2.1 Problem definition

As mentioned above, the main objective of the present

work is to carry out a detailed **finite** **element**

computational investigation of the FSW process.

Since the purpose of the present investigation is to

help establish the basic relationships between the key

process parameters and the joined materials flow, a

relatively simple workpiece and tool geometries are

used (see the next section). Also, since FSW is generally

used for joining aluminium alloys, a prototypical

aluminium alloy/temper AA5083-H321 is

used as the workpiece material. A fairly detailed

description of this alloy and its H321-temper condition

are provided later.

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

4 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

2.2 Geometrical and meshed models

The geometrical models for the workpiece and the

tool are shown in Figs 2(a) and (b). For simplicity, the

workpiece is considered as a single part; i.e. a perfect

clamping condition is assumed. The workpiece is

modelled as a circular solid plate with a radius of

40.0 mm and thickness of 3.0 mm. As will be clarified

later, due to the use of an arbitrary Lagrangian–

Eulerian (ALE) formulation, the circular plate displayed

in Fig. 2(a) effectively represents a circular

region surrounding the tool in an, otherwise, in**finite**ly

long FSW workpiece. The plate is considered to

contain a concentric circular through-the-thickness

hole with a radius of 3.0 mm. The two-part tool is

modelled using a 3.0 mm radius cylindrical pin lower

section and a 9.0 mm radius circular disc-shaped

upper shoulder section. The bottom surface of the

shoulder is not parallel with the workpiece but is

rather inclined at an angle of 80.5 degrees (with

respect to the vertical axis of the tool).

The workpiece is meshed using 9000 first-order

eight-node reduced-integration hexahedral **thermomechanical**ly

**coupled** solid **element**s, while the tool

was meshed using 2000 first-order four-node

reduced-integration rigid shell **element**s. Thermal

properties of the tool are modelled using one singlenode

heat-capacity type of **element**. The meshed

models for the workpiece and the tool are shown in

Figs 3(a) and (b) respectively.

2.3 **Fully** **coupled** **thermomechanical** analysis

To investigate the FSW process, a fully **coupled** **thermomechanical**

**finite** **element** analysis was utilized.

Within this analysis, the nodal degrees of freedom

7.0mm

1.0mm

8.0mm

18.0mm

6.0mm

80.0mm

6.0mm

80.5 º

4.0mm

Fig. 2 Geometrical models with dimensions for (a) the

FSW tool and (b) the FSW workpiece

(a)

(b)

include both the nodal velocities and nodal temperatures.

Furthermore, solid mechanics and heattransfer

aspects of the analysis are two-way/fully

**coupled**; i.e. the work of plastic deformation and that

associated with frictional sliding are considered as

heat sources within the thermal analysis, while the

effect of local temperature on the mechanical aspect

of the analysis is accounted for through the use of

temperature-dependent workpiece material properties.

At the beginning of the computational analysis, the

following (initial) conditions are employed: the tool is

assigned a fixed rotational speed in at a range of

200–400 r/min and a zero translational velocity, while

the workpiece is assumed to be stationary. Both the

tool and the workpiece are initially set to a temperature

of 298 K.

During the analysis, the following boundary conditions

are employed: (a) the bottom of the workpiece

is constrained in the through-the-thickness

direction; (b) the tool rotation is maintained at the

same initial angular velocity; (c) a fixed contact

pressure of 70 MPa is applied over the tool shoulder/

workpiece contact interface; and (d) the workpiece is

not translated along the weldline during the first 2 s.

Thereafter, tool translation along the weldline is

accomplished by applying a constant material flow

velocity in the weldline direction over the in-flow and

out-flow rim surfaces of the workpiece. Heat convection

thermal boundary conditions are applied

over the portions of the workpiece surfaces that

are not in contact with the tool. Typical values for

Fig. 3 Meshed models for (a) the FSW tool and (b) the FSW

workpiece

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

(a)

(b)

the heat transfer coefficient are assigned to the

workpiece/air and to the workpiece/backing plate

interfaces.

To deal with the potential hourglassing problem

associated with the use of reduced integration **element**s

and the incompressible nature of plastic

deformation in the workpiece material, a relaxed

hourglass stiffness method was employed.

The tool and the workpiece are allowed to interact

over their contact surfaces. Specifically, contacts

between the bottom surface of the tool shoulder and

the top surface of the workpiece as well as those

between the outer surface of the pin and the workpiece

hole were considered. Details regarding the

contact algorithm used are provided in section 2.5.

All the calculations are carried out using the commercial

**finite** **element** package ABAQUS/Explicit

[34].

2.4 Material models

As mentioned earlier, the FSW tool is considered to

be rigid and, hence, no mechanical properties (except

for the density) had to be specified for its material.

On the other hand, since the tool was acquiring

a portion of the heat generated as a result

of tool–workpiece interfacial slip, during the FSW

process its thermal capacity had to be specified.

Considering the fact that the tool is often made of a

hot-worked tool steel such as AISI H13, temperatureinvariant

thermal properties and density of this

material were used to compute the thermal capacity

of the tool [35].

As mentioned earlier, the alloy whose FSW behaviour

is analysed in the present work is AA5083-H321.

While often age-hardened Al alloys (e.g. AA6061-T6)

are friction-stir welded, the microstructure evolution

of these alloys during FSW is expected to be substantially

more complex due to the unstable nature of

its precipitates (i.e. precipitates can undergo partial

or complete dissolution during alloy exposure to high

temperature and can reappear upon cooling in different

morphologies and number densities, and even

precipitates with different crystal structures may

appear). AA5083 (nominal chemical composition:

4.5 wt% Mg, 0.25 wt% Cr, 0.75 wt% Mn) is an Mg/Mn

solid–solution hardened alloy and, in addition, in its

H321 temper state is cold work-hardened and stabilized

(to obtain a needed level of ageing/over-ageing

resistance). While Al6Mn precipitates are present in

this alloy, due to the aforementioned stabilizing heat

treatment, they are relatively resistant to both dissolution

and coarsening so that the precipitate portion

of the material microstructure can be taken as

mainly unchanged during FSW.

For the workpiece material, both thermal and

mechanical properties had to be specified. Assuming

Thermomechanical **finite** **element** analysis of material evolution 5

that the workpiece is made of an aluminium alloy

AA5083, the following temperature-invariant and

microstructure-invariant thermal properties were

used: thermal conductivity, k, ¼ 120 W/m K; specific

heat, c p, ¼ 880 J/kg K; and density, r, ¼ 2700 kg/m 3 .

The workpiece material is assumed to behave as an

isotropic linear-elastic and a strain-rate sensitive,

strain-hardenable, and (reversibly) thermally softenable

plastic material. In this type of material, the

mechanical response is described by the following

three relations: (a) a yield criterion, i.e. a mathematical

relation that defines the condition which must

be satisfied for the onset (and continuation) of plastic

deformation; (b) a flow rule, i.e. a relation that

describes the rate of change of different plastic strain

components during plastic deformation; and (c) a

constitutive law, i.e. a relation that describes how the

material strength changes as a function of the extent

of plastic deformation, the rate of deformation, and

temperature. For AA5083 analysed in the present

work, the following specific mechanical model relations

were used:

2.4.1 Yield condition

The von Mises yield condition was used, according to

which the equivalent stress s must be equal to the

material yield strength, sy, i.e.

f ðs 0 ij ; syÞ

q

¼s sy ¼

sy > 0 ð1Þ

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi

ð3=2Þs 0 ij «0 ij

where f is the yield function, s 0 ij and «0 ij denote

respectively the stress and strain components, the

superscript 0 is used to denote deviatoric quantities,

and repeated subscripts imply summation.

2.4.2 Flow rule

The associative/normality flow rule is used in the

present work, according to which the plastic flow

takes place in the direction of the stress gradient of

the yield surface as

_« pl ¼ _ l df

ds0 ð2Þ

ij

where the superscript pl is used to denote a plasticityrelated

quantity, a raised dot denotes a time derivative

and l is a proportionality constant.

2.4.3 Constitutive law

In the present work, the workpiece material yield

strength was assumed to be controlled by strain and

strain-rate hardening as well as by reversible thermally

activated slip-controlled thermal softening

effects. Accordingly, the Johnson–Cook strength

model [36] was used as the basis for constitutive law

in the material under investigation. This model is

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

6 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

capable of representing the material behaviour displayed

under large-strain, high deformation rate,

high-temperature conditions, of the type encountered

in the problem of computational modelling of

the FSW process. Within the Johnson–Cook model,

the yield strength is defined as

sy ¼

h

A þ Bð« pl Þ nih

1 þ C1 logð_« pl =_« pl

0 Þ

ih

1 T m H

i

ð3Þ

where « pl is the equivalent plastic strain, _« pl the

equivalent plastic strain rate, _« pl

0 a reference equivalent

plastic strain rate, A the zero-plastic-strain, unitplastic-strain-rate,

room-temperature yield strength,

B the strain-hardening constant, n the strain-hardening

exponent, C1 the strain-rate constant, m the

thermal-softening exponent, and TH ¼ (T Troom)/ (Tmelt Troom), a room-temperature (Troom) based

homologous temperature while Tmelt is the melting

temperature. All temperatures are given in Kelvin.

A summary of the Johnson–Cook strength model

parameters for AA5083 is provided in Table 1.

While in the original Johnson–Cook strength model

the evolution of the equivalent plastic strain is

assumed to be controlled entirely by the plastic

deformation process, in the present work, plastic

strain evolution is assumed to be controlled by

competition between plastic yielding and dynamic

recrystallization. Since this represents one of the key

contributions of the present work, details regarding

the proposed modifications of the Johnson–Cook

strength model are deferred to the results in the discussion

section, section 3.

2.4.4 Integration of the stress state

During loading, the stress is updated by integrating

the rate form of Hooke’s law

_sij ¼ Cijkl _« el

kl ¼ Cijkl _«kl Cijkl _« pl

kl

ð4Þ

where Cijkl is the fourth-order elastic stiffness tensor

and the total strain rate _« is assumed to be comprised

of its elastic, _« el , and plastic, _« pl , components. At each

step during loading, the total strain rate is known

(computed from the known velocity gradient).

Table 1 Johnson–Cook strength model material parameters

for AA5083-H116

Parameter Symbol Units Value

Reference strength A MPa 167.0

Strain-hardening parameter B MPa 596.0

Strain-hardening exponent n N/A 0.551

Strain-rate coefficient C N/A 0.001

Room temperature Troom K 293

Melting temperature Tmelt K 893.0

Temperature exponent m N/A 1.0

After equation (2) is plugged into equation (4),

equations (1) to (4) constitute a set of eight equations

with eight unknowns ( _sij, _ l, sy). These equations can

be readily solved/integrated using one of the

numerical integration techniques.

2.5 Tool/workpiece interactions/contact

Normal interactions between the tool and the workpiece

were accounted for using a penalty contact

algorithm. Within this algorithm, the penetration of

the surfaces into each other is resisted by linear

spring forces/contact pressures with values proportional

to the depth of penetration. These forces

therefore tend to pull the surfaces into an equilibrium

position with no penetration. Contact pressures

between two bodies are not transmitted unless

the nodes on the slave surface contact the master

surface. There is no limit to the magnitude of the

contact pressure that could be transmitted when the

surfaces are in contact. Transmission of shear stresses

across the contact interfaces is defined in terms of

a static and a kinetic friction coefficient and a stick/

slip critical shear stress level (the maximum value of

shear stress that can be transmitted before the contacting

surfaces begin to slide). In accordance with

standard practice in this field, both the static and the

kinetic friction coefficients are set to a value of 0.3.

The stick/slip critical shear stress level is defined

using a modified Coulomb friction law. Within this

law, there is an upper limit of this quantity, which is

equal to the shear strength of the softer of the two

contacting materials. Thus at each level of the pressure,

the stick/slip critical shear stress level is defined

as the smaller of the following two shear stress values:

(a) the softer material shear strength and (b) a product

of the friction coefficient and the contact pressure.

It should be recognized that both the contact

pressure and the contact shear stress are computed

as part of the complete FSW boundary-value problem.

Frictional slip/sliding at the tool/workpiece contact

interfaces is considered as a potential heat

source. The heat generated per unit contact surface

area per unit time, q, is taken to scale with the magnitude

of the tangential/interface shear stress, t, and

the slip rate, ds/dt, as

q ¼ htðds=dtÞ ð5Þ

where h defines the fraction of the frictional slip

energy that is converted to heat. The heat flux, q, is

then partitioned between the tool and the workpiece.

In the present work, it was assumed that the heat

generated at the tool/workpiece interface is equally

partitioned between the tool and the workpiece.

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

2.6 Explicit solution of the fully **coupled**

**thermomechanical** problem

As mentioned earlier, to analyse the FSW process

computationally, a fully **coupled** **thermomechanical**

**finite** **element** analysis was employed. Within this

analysis the thermal energy conservation equation in

the form

rcp _ T ¼rðkrTÞþhs 0 ij _«pl

ij

and a (dynamic) mechanical equilibrium equation

@sij

@xj

ð6Þ

þ fi ¼ r @2ui ði; j ¼ 1; 2; 3Þ ð7Þ

@t 2

are solved, where ! is a gradient/divergence operator,

x is the spatial coordinate, and f denotes a body

force.

Within ABAQUS/Explicit, equation (7) is integrated

using an explicit forward difference integration

scheme as

Ti þ 1 ¼ Ti þ Dti þ 1Ti

ð8Þ

where subscript i refers to the time-step increment

number. The temperature rate vector, _ Ti, is calculated

at the end of the time increment i as

_Ti ¼ C 1 ðPi FiÞ ð9Þ

where C 1 is the (inverse) lumped thermal capacity

matrix, P the applied source vector, and Fi is the

internal thermal flux vector.

The mechanical equilibrium equation is integrated

using a central difference integration approach as

_u i þ 1=2 ¼ _u i 1=2 þ Dti þ 1 þ Dti

2

_ui þ 1 ¼ ui þ Dti þ 1 _u i þ 1=2

€ui

ð10Þ

ð11Þ

The acceleration vector at the end of the time increment

i is computed as

€u1 ¼ M 1 ðLi IiÞ ð12Þ

where M 1 is the (inverse) mass matrix, Li the applied

load vector, and Ii is the internal force vector.

2.7 Computational cost

Computational investigations of manufacturing/fabrication

processes such as FSW can be very costly/

time consuming. This can particularly become an

issue in the case of explicit **finite** **element** analyses,

which are conditionally stable (i.e. these analyses

entail that the time increment used be smaller than a

critical/stable time increment). In the present fully

**coupled** **thermomechanical** analysis both the

mechanical and the thermal parts of the problem are

associated with their respective stable time incre-

Thermomechanical **finite** **element** analysis of material evolution 7

ments. The overall stable time increment is then

defined as the smaller of the two.

The mechanical stable time increment is generally

defined by the condition that, within the time increment,

the stress wave must not propagate a distance

longer than the minimal dimension of any **finite**

**element** in the mesh. Consequently, the mechanical

stable time increment is defined as Dtmax,mech ¼

lmin/cd, where lmin is the smallest-**element** edge

length, while cd is the dilatational wave propagation

velocity (sound speed), which is defined as

cd ¼ ffiffiffiffiffiffiffiffi p

E=r,

where E is Young’s modulus. For aluminium

alloys, the sound speed, cd, is ca. 5100 m/s and

for the smallest workpiece **element** size used in the

present work ( 0.6 mm), the stable time increment

Dtmax,mech is 1.0 · 10 7 s. For a typical FSW test runs

of 20 s, an explicit **finite** **element** computational

analysis would use 2 · 10 8 time increments. Using

the computational facilities available for the present

work, this would require an estimated computational

wall time of 96 hours per single computational analysis.

Since this computational cost was unacceptably

high, a mass-scaling algorithm was used. Within this

algorithm, material density is artificially increased in

order to increase the stable time increment. The use

of such a mass scaling algorithm does not alter the

amount of heat generated by dissipation of plastic

deformation work and frictional slip. Also, care was

taken to ensure that a kinetic energy over internal

energy ratio is less than 1 per cent, which is recommended

in order to ensure that the mechanical

portion of the solution is not altered by mass scaling.

The thermal stable time increment is generally

defined by the condition that, within the time increment,

the thermal wave must not propagate a

distance longer than the minimal dimension of

any **finite** **element** in the mesh. Consequently,

the thermal stable time increment is defined as

Dtmax,therm ¼ lmin 2 /(2a), where lmin is the smallest**element**

edge length, while a is the thermal diffusivity.

Using the aforementioned thermal property

values for AA5083, the thermal stable time increment

has been computed as Dtmax,therm is 1.0 · 10 3 s. It

should be noted that the mass scaling algorithm used

does not affect this stable time increment and that

the modified mechanical stable time increment does

not exceed the thermal stable time increment. Consequently,

mass scaling does not affect the thermal

portion of the fully **coupled** **thermomechanical**

problem investigated in the present work.

2.8 Arbitrary Lagrangian–Eulerian (ARL)

formulation

As established earlier, FSW involves extensive plastic

deformation and large-scale motion of the material

from the region in front of the tool to the region

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

8 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

behind the tool. Under such conditions, the pure

Lagrangian formulation in which the **finite** **element**

mesh is attached to the material and moves/deforms

with it can encounter serious numerical difficulties.

To overcome this problem, the **finite** **element** analysis

of the FSW process carried out in the present work

was based on the so-called arbitrary Lagrangian–

Eulerian (ALE) formulation. Within this algorithm,

adaptive remeshing is carried out during a computational

run to ensure that the mesh remains of a

high quality. This approach is generally preferred

over the pure Eulerian formulation in which the

mesh remains unchanged/stationary while the

material flows through it. Since the ALE mesh has a

Lagrangian character, it can readily track material

surfaces and prevent the formation of partially filled

**element**s. The latter two problems are often cited as

key shortcomings of the pure Eulerian formulation.

The ALE formulation used in the present work

involved the following three main aspects:

(a) The workpiece mesh is assumed to be stationary

(i.e. of the Eulerian type) in the circumferential

direction, while in the radial and in the throughthe-thickness

directions the same mesh is

allowed to follow the material (i.e. the mesh is

assumed to be of the Lagrangian type).

(b) The inflow and outflow rim surfaces of the

workpiece plate are treated as being pure

Eulerian, and thus stationary.

(c) The top and bottom workpiece plate surfaces are

treated as being of the sliding type; i.e. the mesh

is allowed to follow the material in the direction

normal to the surface but remains stationary in

the other two orthogonal directions.

3 RESULTS AND DISCUSSION

3.1 Material model modification to include the

effects of dynamic recrystallization

As mentioned earlier, the workpiece material

AA5083-H321 is modelled using a modified Johnson–

Cook strain-hardening, strain-rate-sensitive, temperature-softening

yield-strength model. Within the

original Johnson–Cook model of equation (3), temperature

provides only a reversible effect in promoting

plastic deformation via thermal activation of

dislocation glide and climb. Simply stated, higher

temperatures promote plastic yielding but, per se,

are not considered to (irreversibly) alter material

microstructure/properties. However, as pointed out

earlier, during FSW the workpiece material in the

weld/stir zone becomes heavily plastically deformed

and it is generally subjected to temperatures very

near, yet lower than, the material melting tempera-

ture. Under these conditions, the material tends to

undergo annealing at the same time as it is being

deformed plastically. In other words, the material in

the stir/nugget region tends to dynamically recrystallize,

as a result of which the material strength/

hardness (at high welding temperatures as well as at

room temperature) is lowered relative to that in the

base (H321 temper condition) material. This effect of

temperature is not accounted for in the original

Johnson–Cook model. Rather, only the effect of high

temperatures on promoting plastic deformation via

thermal activation is taken into account.

To overcome the aforementioned deficiency of the

original Johnson–Cook model, a modification is proposed

to the differential equation governing the

evolution of the equivalent plastic strain. In the

original Johnson–Cook model, this evolution was

governed by simultaneously satisfying Hooke’s law,

yield criterion, and flow rule relations (see section

2.4). In this way, only the effect of strain hardening

due to an increase in the dislocation density and the

resulting increase in the dislocation motion resistance

imposed by the surrounding dislocations is

taken into account. To include the effects of dynamic

recrystallization, a simple phenomenological-based

relation for the additional (negative) component in

the equivalent plastic strain rate is proposed. This

equation is based on the following physics-based

arguments:

(a) Dynamic recrystallization is a thermally activated

process and consequently the correction term in

the equivalent plastic strain evolution equation

must contain a Boltzmann probability term in

the form exp( Q/RT ), where Q is an activation

energy while R is the universal gas constant. In

other words, the dynamic recrystallization correction

to the Johnson–Cook strength model

should be an Arrhenius-type function.

(b) Since the rate of recrystallization across various

alloy systems appears to scale with the dimensionless

absolute-zero-based homologous temperature,

Th (defined as the ratio of the

temperature and the melting temperature, both

temperatures expressed in K), it is convenient to

replace the Q/RT term in the Boltzmann probability

relation with q/Th, where q is a dimensionless

activation energy.

(c) Due to the fact that the rate at which material

tends to recrystallize increases as the amount of

cold work is increased, q should be a decreasing

function of the equivalent plastic strain «pl.

Based on these arguments, the dynamic recrystallization

contribution to the evolution of the

equivalent plastic strain can be expressed as

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

_« pl;dyn rec ¼ _« 0;pl;dyn rece qð« ð plÞ=ThÞ ð13Þ

where _« 0;pl;dyn rec is a dynamic recrystallization

frequency/preexponential term. An analysis of the

available experimental data pertaining to the kinetics

of recrystallization of AA5083 [37] showed that q

scales inversely with «pl raised to a power of 2.9.

Based on this finding and using the curve-fitting

results for the experimental recrystallization–kinetics

data reported in reference [37], it is found that

equation (13) can be rewritten as

_« pl;dyn rec ¼ 21:5e

1=ð« 2:9

pl T hÞ

ð14Þ

The effect of equation (14) on modifying the

behaviour of AA5083 under simple uniaxial tensile

conditions is displayed in Figs 4(a) to (c). In Fig. 4(a),

it is seen that when Th is relatively low (Th ¼ 0.3), the

effects of dynamic recrystallization are small so that

the material strain hardens. In sharp contrast, when

Th is relatively high (Th ¼ 0.9), the effect of dynamic

recrystallization is dominant so that, despite extensive

plastic deformation, the material undergoes

pronounced strain softening (Fig. 4(b)). In Fig. 4(c), it

is seen that when the effects of strain hardening and

dynamic recrystallization are comparable, at the

intermediate values of Th (Th ¼ 0.5) no significant

change in material strength takes place during plastic

deformation.

The oscillating behaviour of material strength seen

in Fig. 4(c) is a result of the competition and the

interaction between strain hardening and dynamic

recrystallization induced softening processes; i.e.

softer material tends to harden at a high rate and,

when the amount of plastic strain in the workpiece

becomes sufficiently large, the rate of dynamic

recrystallization becomes high enough to bring the

strength down. This type of oscillating strength

behaviour is often a signature of the undergoing

dynamic recrystallization process.

It should be recognized that the kinetics of recrystallization

is generally described using the so-called

Johnson–Mehl–Avrami equation (e.g. reference [38]).

Within this equation, the volume fraction of the

material recrystallized, as a function of time, is given

by a characteristic S-shaped curve, which starts from

a non-zero annealing time (the incubation period),

increases with a higher and higher slope, and, ultimately,

the slope decreases as the volume fraction of

the recrystallized material approaches unity (Fig. 5).

The inner steepest part of this curve generally covers

the major portion (80–90 per cent) of the range of the

recrystallized material volume-fraction. Taking this

fact into account, the simple model proposed here

assumes that the entire recrystallized material

volume-fraction versus time curve can be represented

by its inner part and that this portion can be

Thermomechanical **finite** **element** analysis of material evolution 9

Strength,

MPa

d

l

e

i

Y

Strength,

MPa

d

l

e

i

Y

a

P

M

,

h

t

g

n

e

r

t

S

d

l

e

i

Y

570

560

550

540

530

520

510

500

560

540

520

500

480

460

440

420

580

560

540

520

500

480

460

(a)

Original Johnson Cook Model

Modified Johnson Cook Model

1 2 3 4 5 6 7

Equivalent Plastic Strain

(b)

Th=0.3

Th=0.9

Original Johnson Cook Model

Modified Johnson Cook Model

1 2 3 4 5 6 7

Equivalent Plastic Strain

(c)

Th=0.5

Original Johnson Cook Model

Modified Johnson Cook Model

1 2 3 4 5 6 7

Equivalent Plastic Strain

Fig. 4 A comparison of the strength versus equivalent

plastic strain curves as predicted by the original and

the modified Johnson–Cook strength models. The

results are obtained under the uniaxial strain rate of

0.001/s and at three different homologous temperatures:

(a) u ¼ 0.3; (b) u ¼ 0.9; (c) u ¼ 0.5

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

10 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

Fraction

Recrystali

zed

1

0.8

0.6

0.4

0.2

0

10 1

10 2

Annealing Time, sec

linearized. The slope of this new linear function, on

the other hand, is taken to be a function of the temperature

and the equivalent plastic strain. Equation

(14) is then obtained by assuming that _« pl;dyn rec

scales linearly with the rate of recrystallization.

To include the effects of dynamic recrystallization

of the workpiece material on the material evolution

during FSW, the modified Johnson–Cook material

model is implemented into a user material subroutine

VUMAT.for and linked with the ABAQUS/

Explicit **finite** **element** solver. To validate the implementation

of the material model, several FSW cases

were analysed. It is found that when the effects of

dynamic recrystallization are suppressed, the results

(not shown for brevity), based on the user material

model and the Johnson–Cook model (built in ABA-

QUS/Explicit) are essentially identical.

3.2 Typical computational results

In this section, examples of typical results obtained in

the fully **coupled** **finite** **element** investigation of the

FSW process carried out in this work are presented

and discussed. The **finite** **element** analysis used

allowed investigation of the effect of all the key FSW

process parameters on the temporal evolution and

spatial distribution of various material-related

quantities such as: temperature, stress and strain

components, equivalent plastic strain, local material

strength, material velocity, trajectory of tracer

particles that reveal temporal-dependent locations of

the associated material particles as they are passing

through the circular region surrounding the rotating

pin tool, etc. Since similar results were shown and

discussed in a series of papers by Zhang et al. [29–31],

10 3

Fitted, 773K

Fitted, 573K

Experimental [37], 773K

Experimental [37], 573K

Fig. 5 Experimental results [37] and the fitting curves

pertaining to the recrystallization kinetics in AA5083

10 4

10 5

In-flow

In-flow

In-flow

Hole

Transverse

Section

Outflow

only a few representative and unique results will be

displayed and discussed in this section.

3.2.1 Nodal velocity field

The distribution of nodal velocities at the outer surfaces

of the workpiece at two different times (0.0 and

0.5 s) is displayed in Figs 6(a) and (b). For clarity, the

tool is not shown in Figs 6(a) and (b), as well as in

several other figures presented in the remainder of

this document. These figures clearly show that the

initially assigned unidirectional velocity field in the

(a)

Outflow

Fig. 6 A typical nodal-velocity field associated with friction

stir welding: (a) the initial state; (b) the fully developed

state; (c) a close-up of part (b); and (d) a closeup

of the transverse section of part (b)

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

(b)

(c)

(d)

Q4

direction of welding quickly transforms into the

velocity field in which there is a well-defined stir

region right below the shoulder (within which the

material circles around the pin) and the remainder of

the field (within which the material tends to flow

around the stir region). A comparison of the results

displayed in Figs 6(a) and (b) clearly shows how the

region underneath the tool shoulder, which is initially

unfilled, becomes filled as FSW proceeds (please

note an increase in the workpiece hole upper rim

altitude). Once the space under the shoulder is fully

filled it remains filled as the FSW process continues.

The material in this region is constantly being refreshed

as the tool advances in the welding direction. To

reveal the character of the nodal velocity field around

the workpiece hole better, a close-up of this region is

provided in Fig. 6(c). Furthermore, to reveal the toolinduced

material stirring effect through the workpiece

thickness, a transverse section of the plate is

provided in Fig. 6(d).

3.2.2 Material/tracer particle trajectories

The results displayed in Figs 6(a) and (b) show the

spatial distribution and temporal evolution of the

nodal velocities. It should be noted that due to the

ALE character of the **finite** **element** analysis used in

the present work, the motion of the **finite** **element**

mesh is not completely tied to the motion of the

material. Thus the results displayed in Figs 6(a) and

(b) show the velocities of the material particles,

which at that moment pass through the nodal points.

However, at different times different material particles

are associated with the same nodes. To observe

material extrusion around the tool pin and its forging

at the tool wake, it is more appropriate to construct

and analyse material particle trajectories. This is

possible within ABAQUS/Explicit through the use of

so-called tracer particles, which are attached to the

material points (and not to the mesh nodal points).

An example of the prototypical results pertaining to

the trajectory of retreating-side and advancing-side

tracer particles is displayed in Figs 7(a) and (b)

respectively. The tracer particles displayed in these

figures are initially located in a plane that is halfway

between the top and bottom surfaces of the workpiece.

For improved clarity, tracer particle trajectories

are colour coded. The results displayed in

Figs 7(a) and (b) clearly revealed the following basic

aspects of the FSW process:

(a) The workpiece material at the retreating side (as

represented by the yellow and green tracer particle

trajectories in Fig. 7(a)), does not, for the

most part, enter the stir zone under the tool

shoulder and usually only flows around it.

(b) The material at the advancing side (as represented

by the white and cyan tracer particle

Thermomechanical **finite** **element** analysis of material evolution 11

trajectories in Fig. 7(b)), which is initially close to

the butting surfaces, passes over to the retreating

side and is co-stirred with some of the retreatingside

material to form the welded joint.

(c) The advancing-side material further away from

the initial butting surfaces remains on the

advancing side and either enters the stir region

on the advancing side or flows around it.

3.2.3 Temperature field

A typical spatial distribution of temperature in the

workpiece during FSW is displayed in Figs 8(a) and

(b). The results displayed in Figs 8(a) and (b) refer to

the temperature distributions over the medial longitudinal

and medial transverse sections respectively.

Simple examination of the results displayed in these

figures and of the results obtained in the present

work (but not shown for brevity) reveals that:

(a) Depending on the FSW process conditions such

as tool contact pressure, tool rotational and

translational speeds, temperatures in a range

between 350 and 450 C are obtained.

(b) The highest temperatures are always found in the

workpiece material right below the tool shoulder

and the temperatures progressively decrease

from this region as a function of the distance in

the radial and through-the-thickness directions.

(c) As the tool rotational speed and contact pressure

are increased, higher temperatures are observed

and temperature differences between the top and

bottom surfaces of the workpiece are reduced.

In-flow

Retreating Side

Advancing Side

In-flow

Fig. 7 (a) Retreating-side and (b) advancing-side tracer

particle typical trajectories

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

(a)

(b)

Q7

12 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

In-flow

(a)

(b)

(c)

In-flow

Outflow

Outflow

Fig. 8 Typical temperature distribution over one-half of

the workpiece obtained by cutting along (a) the

longitudinal and (b), (c) transverse directions:

maximum (red) ¼ 400 C; minimum (blue) ¼ 25 C

(d) By computing the energies dissipated via the

plastic deformation process and those dissipated

through frictional sliding at the tool/workpiece

interfaces, it is found that plastic deformation

typically contributes around 30 per cent to the

overall heat generation and that this contribution

increases slowly with an increase in the translational

velocity of the tool.

3.2.4 Equivalent plastic strain field

A typical spatial distribution of equivalent plastic

strain in the workpiece during FSW is displayed in

Figs 9(a) and (b). The results displayed in Figs 9(a)

and (b) refer to the equivalent plastic strain distributions

over the medial longitudinal and medial

transverse sections respectively. Simple examination

of the results displayed in these figures and of the

results obtained in the present work (but not shown

for brevity) reveals that:

In-flow

(a)

(b)

In-flow

Outflow

Fig. 9 Typical equivalent plastic strain distribution over

one-half of the workpiece obtained by cutting along

(a) the longitudinal and (b) transverse directions:

maximum (red) ¼ 120; minimum (blue) ¼ 0

(a) Depending on the FSW process conditions, such

as tool contact pressure, tool rotational and

translational speeds, equivalent plastic strains in

a range between 100 and 150 are observed. This

range of equivalent plastic strains is in general

agreement with the ones previously reported by

Zhang and co-workers (e.g. references [17] and

[27]to[31]. It should be noted that the workpiece

material is capable of undergoing such a large

amount of plastic deformation due to the

attendant high-pressure conditions. Such highpressure

conditions are normally not present

in standard laboratory mechanical tests (e.g.

uniaxial tension, compression, simple shear,

etc.), which are used to parameterize the

workpiece material model. Consequently, the

results obtained in these tests reflect the material

behaviour under significantly lower levels of the

plastic strain and, as is generally done, it is

assumed here that the established material

model identification can be extrapolated into the

extremely large equivalent plastic-strain range

encountered in the FSW process.

(b) The highest equivalent plastic strains are always

found in the workpiece material right below the

tool shoulder and equivalent plastic strains

progressively decreased from this region as a

function of the distance in the radial and

through-the-thickness directions.

(c) There is a highly pronounced asymmetry in the

distribution of the equivalent plastic strain relative

to the initial location of the butting surfaces.

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

This asymmetry is related to the aforementioned

differences in the material transport (at the

advancing and the retreating sides of the weld)

from the region ahead of the tool to the region

behind the tool.

(d) As the tool translational speed is decreased

and the tool/workpiece contact pressure is

increased, higher equivalent plastic strains are

observed and equivalent plastic strain differences

between the top and bottom surfaces of

the workpiece are reduced. This finding suggests

that under these FSW process conditions the

extent of material stirring/mixing (which plays a

critical role in weld quality/joint strength) is

increased.

3.2.5 Residual stress field

It is well established that friction-stir welded

components contain significant levels of residual

stresses, both in the direction of welding (the longitudinal

direction) and in the direction normal to it

(the transverse direction). These residual stresses are

caused by non-uniform distributions in the extent of

plastic deformations (as represented by the

equivalent plastic strains) and in the temperature in

different regions within the weld joint. Since the

presence of residual stresses can significantly affect

the structural and environmental resistance/durability

of welded joints, it is critical that they are

quantified and that their magnitudes and spatial

distributions be correlated with various FSW process

parameters. While a comprehensive investigation of

the residual stress distribution as a function of the

FSW process parameters is beyond the scope of the

present work, an effort was invested here to develop

computational capabilities for such investigations.

Towards that end, the results of the FSW simulation

are imported into the implicit **finite** **element** program

ABAQUS/Standard and a quasi-static fully **coupled**

**thermomechanical** analysis is carried out. It should

be noted that ABAQUS/Explicit is not suitable for this

type of investigation since it requires prohibitively

long computational times. Within the quasi-static

fully **coupled** **thermomechanical** analysis employed,

the FSW tool is removed and the boundary conditions

are eliminated from the workpiece while the

temperature is progressively decreased down to room

temperature.

An example of the results pertaining to the distribution

of von Mises residual stresses over a

medial longitudinal and transverse sections of the

workpiece are displayed in Figs 10(a) and (b)

respectively. Simple examination of the results displayed

in these figures and of the results obtained

in the present work (but not shown for brevity)

reveals that:

Thermomechanical **finite** **element** analysis of material evolution 13

In-flow

(a)

(b)

In-flow

Outflow

Fig. 10 Typical von Mises residual stress distribution over

one-half of the workpiece obtained by cutting

along (a) the longitudinal and (b) transverse

directions: maximum (red) ¼ 50 MPa; minimum

(blue) ¼ 20 MPa

(a) Maximum longitudinal residual stresses are generally

higher than their maximum transverse

counterparts by a factor of roughly two

(b) The residual stresses typically increase in magnitude

as the distance from the initial portion of

butting surfaces is reduced. However, in the

innermost portion of the nugget, they tend to

decrease somewhat. This is clearly related to the

effect of dynamic recrystallization, which is prevalent

in this region.

(c) Both the longitudinal and transverse residual

stresses tend to increase with an increase in the

tool rotational and translational velocities.

3.3 Comparison with experimental results

The results presented in the previous section (as well

as the results obtained in the present work but not

shown) are very reasonable and in good qualitative

agreement with the general experimental observations/findings.

However, if the computational

approach like the one developed here is to become an

integral part of the FSW practice and helps guide

further development and optimization of this metal

joining process, it must also demonstrate the needed

level of quantitative agreement with the experimental

results/observations. To assess the ability of the present

computational approach to account for the

experimentally measured FSW-related results, selected

computational results are compared with their

experimental counterparts obtained in the work of

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

14 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

Peel et al. [26]. The work carried out in reference [26]

is quite comprehensive and thorough and involves

AA5083, the aluminium alloy investigated in the

present work. While the work of Peel et al. [26] yielded

numerous results, only the following two types of

these results could be directly compared with the

**finite** **element** based computational results obtained

in the present work: (a) variation of the longitudinal

and transverse (normal) residual stresses as a

function of the distance from the weldline and (b)

variation of the room temperature material strength

as a function of the distance from the weldline.

3.3.1 Residual stress distribution

A comparison between the present computed and

the experimentally measured results reported in

reference [26] pertaining to variation of the longitudinal

and transverse residual stresses as a function

of the distance from the initial location of the butting

surfaces is displayed in Figs 11(a) and (b). Two sets of

computational results are displayed in each case, one

using the original Johnson–Cook model and the other

using the modified Johnson–Cook model. This

helped establish the extent of improvement in the

material model formulation attained in the present

work. Simple examination of the results displayed in

Figs 11(a) and (b) reveals that the results obtained

using the modified Johnson–Cook model is in

significantly better agreement (than the original

Johnson–Cook-based results) with the experimental

results, making the overall computation/experiment

agreement quite good. Specifically:

(a) The residual stresses are compressive at larger

distances from the weldline at the advancing

side of the weld (the right-hand side in Figs 11(a)

and (b)).

(b) As the weldline at the advancing side is approached,

the residual stresses first increase in magnitude

and then switch their character (i.e.

become tensile), at a distance of 15–20 mm from

the weldline (at the advancing side).

(c) In the innermost portion of the nugget, the tensile

residual stresses tend to decrease somewhat.

(d) As the distance from the weldline increases

on the retreating side, the stresses gradually

decrease towards zero.

(e) The longitudinal residual stresses are generally

higher than their transverse counterparts.

3.3.2 Room-temperature material strength

distribution

A comparison between the present computed results

(as predicted by the modified and the original Johnson–Cook

strength model) and the experimentally

measured results reported in reference [26] pertain-

Stress,

MPa

l

a

n

i

d

u

t

i

g

n

o

L

Residual

Stress,

MPa

e

s

r

e

v

s

n

a

r

T

Residual

60

40

20

0

-20

-40

40

30

20

10

0

-10

-20

Original Johnson-Cook

Modified Johnson-Cook

Experimental [42]

-10 0 10 20 30 40

Lateral Distance from Weld-line, mm

Original Johnson-Cook

Modified Johnson-Cook

Experimental [42]

-10 0 10 20 30 40

Lateral Distance from Weld-line, mm

(a)

(b)

Fig. 11 Variation of (a) the longitudinal and (b) transverse

residual stresses as a function of the distance

from the weldline. Data pertaining to the advancing

side of the weld joint are on the right-hand

side of the plot

ing to variation of the room temperature material

strength as a function of the distance from the initial

location of the butting surfaces is displayed in Fig. 12.

The results displayed in this figure show that, while

the quantitative agreement between the computed

and the experimental results is only fair, the present

computed analysis correctly predicts the overall

trend. This is quite encouraging considering the fact

that the original Johnson–Cook strength model (in

which the effect of dynamic recrystallization is

neglected) incorrectly predicts that the highest room

temperature strength levels are located in the

innermost region of the nugget zone (where the

equivalent plastic strain levels are also the highest).

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

Q5

Strength,

MPa

Room-tempe

rature

260

240

220

200

180

160

140

120

Original Johnson-Cook

Modified Johnson-Cook

Experimental [42]

-15 -10 -5 0 5 10 15

Lateral Distance from Weld-line, mm

Fig. 12 Variation of the room-temperature material

strength as a function of the distance from

the weldline. Data pertaining to the advancing

side of the weld joint are on the right-hand side of

the plot

3.3.3 Material microstructure evolution

In the previous two sections, spatial variations within

the FSW joint, in the residual stresses, and in the

material strength were computed and compared

with their experimental counterparts obtained in

reference [26]. The material strength results were

obtained by substituting the effective (i.e. dynamicrecrystallization

modified) equivalent plastic strain in

the Johnson–Cook strength model of equation (3).

Within this approach, contributions of various

microstructural features/processes (e.g. grain size,

dislocation density, dispersoid number density, etc.)

were lumped into a single parameter, the effective

equivalent plastic strain. In ongoing work, an effort

is made to identify and quantify separately

the contributors to material strength (primarily the

effect of grain size refinement and dislocation density-controlled

strain hardening). In the approach

used, separate evolution equations are being developed

for both the grain size and the dislocation density,

and the standing Hall–Petch grain-size-based

strengthening [38] and Cocks, Argon, and Ashby

strain-hardening models [39] are being utilized. An

example of the preliminary results obtained in this

investigation is displayed in Fig. 13, in which variation

of the grain size as a function of the distance from the

weld centre-line are displayed. These results are

highly encouraging since they show a recrystallized

fine-grain microstructure in the nugget zone and a

somewhat coarser grain microstructure in the heataffected

zone (HAZ), which is consistent with the

Thermomechanical **finite** **element** analysis of material evolution 15

Size,

microns

n

i

a

r

G

50

45

40

35

30

25

20

15

HAZ

-20 -15 -10 -5 0 5 10 15 20

Lateral Distance from Weld-line, mm

typical findings made in the microstructural investigation

of the FSW joints (e.g. reference [26]).

4 CONCLUSIONS

Computational

Nugget

Region

HAZ

TMAZ TMAZ

Fig. 13 Spatial variation of the grain size throughout the

FSW joint as obtained computationally in ongoing

work

Based on the work presented and discussed in the

present work, the following main summary remarks

and conclusions can be made:

1. A comprehensive fully **coupled** **thermomechanical**

**finite** **element** computational

investigation of friction stir welding (FSW) of a

prototypical solid–solution strengthened and

strain-hardened aluminium alloy (AA5083) is

carried out.

2. To model the microstructure/property evolution

of this material during the FSW process, the original

Johnson–Cook strength model is modified in

order to account for the effects of dynamic

recrystallization and the associated material

softening taking place in the stir zone of the

welded joint.

3. Various results obtained showed good overall

qualitative agreement with the corresponding

empirical findings/observations.

4. Limited quantitative experimental results pertaining

to the variations of the longitudinal and

transverse residual stresses with distance from

the weldline and the associated variations in

material strength are used to validate the modified

Johnson–Cook **finite** **element** procedure

employed. A reasonably good agreement is

obtained between the computed and experimental

results, suggesting that the modelling and

simulation procedures used are adequate.

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

16 M Grujicic, T He, G Arakere, H V Yalavarthy, C-F Yen, and B A Cheeseman

ACKNOWLEDGEMENTS

The material presented in this paper is based on

work supported by the US Army/**Clemson** **University**

Cooperative Agreements W911NF-04-2-0024 and

W911NF-06-2-0042.

Ó Authors 2010

REFERENCES

1 Thomas, W. M., Nicholas, E. D., Needham, J. C.,

Murch, M. G., Temple-Smith, P., and Dawes, C. J.

Friction stir butt welding, International Patent

Application PCT/GB92/02203, 1991.

2 Dawes, C. J. and Thomas, W. M. Friction stir process

welds aluminum alloys. Welding J., 1996, 75, 41–52.

3 Thomas, W. M. and Dolby, R. E. Friction stir welding

developments. In Proceedings of the Sixth International

Conference on Trends in Welding Research

(Eds S. A. David, T. DebRoy, J. C. Lippold, H. B. Smartt,

and J. M. Vitek), 2003, pp. 203–211 (ASM International,

Materials Park, Ohio).

4 Cho, J. H., Boyce, D. E., and Dawson, P. R. Modeling

strain hardening and texture evolution in friction stir

welding of stainless steel. Mater. Sci. Engng A, 2005, 398,

146–163.

5 Liu, H., Fulii, H., Maeda, M., and Nogi, K. Tensile

properties and Fracture locations of friction-stir welded

joints of 6061-T6 aluminium Alloy. J. Mater. Sci. Lett.,

2003, 22, 1061–1063.

6 Lee, W. B., Lee, C. Y., Chang, W. S., Yeon, Y. M., and

Jung, S. B. Microstructural investigation of friction stir

welded pure titanium. Mater. Lett., 2005, 59, 3315–3318.

7 Thomas, W. M. and Nicholas, E. D. Friction stir welding

for the transportation industries. Mater. Des., 1997, 18,

269–273.

8 Su, J. Q., Nelson, T. W., Mishra, R., and Mahoney, M.

Microstructural investigation of friction stir welded

7050-T651 aluminum. Acta Mater., 2003, 51, 713–729.

9 Frigaard, O., Grong, Ø., and Midling, O. T. A process

model for friction stir welding of age hardening aluminum

alloys. Metall. Mater. Trans. A, 2001, 32, 1189–1200.

10 Mahoney, M. W., Rhodes, C. G., Flintoff, J. G.,

Spurling, R. A., and Bingel, W. H. Properties of frictionstir-welded

7075 T651 aluminum. Metall. Mater. Trans. A,

1998, 29, 1955–1964.

11 Rhodes, C. G., Mahoney, M. W., Bingel, W. H.,

Spurling, R. A., and Bampton, C. C. Effect of friction stir

welding on microstructure of 7075 aluminum. Scripta

Mater., 1997, 36, 69–75.

12 Liu, G., Murr, L. E., Niou, C. S., McClure, J. C., and

Vega, F. R. Microstructural aspects of the friction-stirwelding

of 6061-T6 aluminum. Scripta Mater., 1997, 37,

355–361.

13 Jata, K. V. and Semiatin, S. L. Continuous dynamic

recrystallization during friction stir welding. Scripta

Mater., 2000, 43, 743–748.

14 Masaki, K., Sato, Y. S., Maeda, M., and Kokawa, H.

Experimental simulation of recrystallized microstructure

in friction stir welded Al alloy using a plane-strain

compression test. Scripta Mater., 2008, 58, 355–360.

15 Thomas, W. M., Nicholas, E. D., Needham, J. C.,

Murch, M. G., Templesmith, P., and Dawes, C. J.

Friction stir welding. International Patent Application

PCT/GB92102203 and Great Britain Patent Application

9125978.8, 1991.

16 Mishra, R. S. and Ma, Z. Y. Friction stir welding and

processing. Mater. Sci. Engng Rep., 2005, 50, 1–78.

17 Zhang, H. W., Zhang, Z., and Chen, J. T. The **finite**

**element** simulation of the friction stir welding process.

Mater. Sci. Engng A, 2005, 403, 340–348.

18 Ramirez, A. J. and Juhas, M. C. Microstructural

evolution in Ti–6Al–4V friction stir welds. Mater. Sci.

Forum, 2003, 426–432.

19 Su, J. Q., Nelson, T. W., Mishra, R., and Mahoney, M.

Microstructural investigation of friction stir welded

7050-T651 aluminium. Acta Mater., 2003, 51, 713–729.

20 Salem, H. G., Reynolds, A. P., and Lyons, J. S.

Microstructure and retention of superplasticity of friction

stir welded superplastic 2095 sheet. Scripta Mater.,

2002, 46, 337–342.

21 Liu, H. J., Chen, Y. C., and Feng, J. C. Effect of zigzag

line on the mechanical properties of Friction Stir

Welded Joints of an Al–Cu Alloy. Scripta Mater., 2006,

55, 231–234.

22 Ma, Z. Y., Sharma, S. R., and Mishra, R. S. Effect of

friction stir processing on the microstructure of

cast A356 aluminum. Mater. Sci. Engng A, 2006, 433,

269–278.

23 Cavaliere, P., Campanile, G., Panella, F., and

Squillace, A. Effect of welding parameters on mechanical

and microstructural properties of AA6056 joints

produced by friction stir welding. J. Mater. Process.

Technol., 2006, 180, 263–270.

24 Cavaliere, P., Squillace, A., and Panella, F. Effect of

welding parameters on mechanical and microstructural

properties of AA6082 joints produced by friction stir

welding. J. Mater. Process. Technol., 2008, 200, 364–372.

25 Elangovan, K. and Balasubramanian, V. Influences of

tool pin profile and welding speed on the formation of

friction stir processing zone in AA2219 aluminium alloy.

J. Mater. Process. Technol., 2008, 200, 163–175.

26 Peel, M., Steuwer, A., Preuss, M., and Withers, P. J.

Microstructure, mechanical properties and residual

stresses as a function of welding speed in aluminium

AA5083 friction stir welds. Acta Mater., 2003, 51,

4791–4801.

27 Zhang, H. W., Zhang, Z., and Chen, J. T. 3D Modeling of

material flow in friction stir welding under different

process parameters. J. Mater. Process. Technol., 2007,

183, 62–70.

28 Zhang, Z., Chen, J. T., and Zhang, H. W. The 3D

simulation of friction stir welding process. In International

Conference on Mechanical engineering and

mechanics (Eds R. C. Batra, L. F. Qian, Y. L. Zhang,

X. N. Li, and S. K. Tso), Nanjing, People’s Republic of

China, 2005, pp. 1388–1342.

29 Zhang, H. W. and Zhang, Z. Numerical modeling of

friction stir welding process by using rate-dependent

Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture JEM1750

constitutive model. J. Mater. Sci. Technol., 2007, 23,

73–80.

30 Zhang, H. W., Zhang, Z., Bie, J., Zhou, L., and Chen,

J. T. Effect of viscosity on material behaviors in friction

stir welding process. Trans. Nonferr. Metal Soc. China,

2006, 16, 1045–1052.

31 Zhang, H. W. and Zhang, Z. Numerical simulation of

friction stir welding by using semi-**coupled** model. In

International Conference on Enhancement and promotion

of computational methods in engineering

science and mechanics (Eds P. Hu and J. N. Reddy),

Changchun, China, 10–12 August 2006, pp. 52–62.

32 Deng, X. M. and Xu, S. W. Two-dimensional **finite**

**element** simulation of material flow in friction stir

welding process. J. Manuf. Process., 2004, 6, 125–133.

33 Xu, S., Deng, X., Reynolds, A. P., and Seidel, T. U. Finite

**element** simulation of material flow in friction stir

welding. Sci. Technol. Weld Joint, 2001, 6, 191–193.

Thermomechanical **finite** **element** analysis of material evolution 17

34 ABAQUS Version 6.8-1, User Documentation, Dassault

Systems, 2008.

35 Ashby, M. F. Materials selection in mechanical design,

edition 3, 2005 (Elsevier Butterworth Heinemann,

Oxford).

36 Johnson, G. R. and Cook, W. H. A constitutive model

and data for metals subjected to large strains, high

strain rates and high temperatures. In Proceedings of

the 7th International Symposium on Ballistics, 1983.

37 Kannan, K., Vetrano, J. S., and Hamilton, C. H. Effects

of alloy modification and **thermomechanical** processing

on recrystallization of Al-Mg-Mn alloys. Metallurg.

Mater. Trans., 1996, 27A, 22–33.

38 Reed-Hill, R. E. Physical metallurgy principles, 1994

(PWS Publishing Company, Boston, Massachusetts).

39 Kocks, U. F., Argon, A. S., and Ashby, M. F.

Thermodynamics and kinetics of slip. Prog. Mater. Sci.,

1975, 19, 1.

JEM1750 Proc. IMechE Vol. 224 Part B: J. Engineering Manufacture

Q6

IMECHE

JOURNAL………JEM ARTID…JEM_1750

TO: CORRESPONDING AUTHOR

AUTHOR QUERIES - TO BE ANSWERED BY THE AUTHOR

The following queries have arisen during the typesetting of your manuscript. Please

answer these queries by marking the required corrections at the appropriate point in the

text.

Query

number

Q1

Q2

Q3

Q4

Q5

Q6

Q7

Query Details

No keywords included. Are these OK?

Refs 9-12 are not cited. Please put in (note order may have to change

if they are not in sequence and see AQ3)

Refs 24-28 not cited. Please put in. However note that 27 and 28 are

mentioned later with Fig. 9 and 26 is in Sec 3.3., 3.3.1, 3.3.2 and 3.3.3.

It will really throw the order out if they are not mentioned earlier

together.

Colour is mentioned in list for Fig. 7 (a) and (b) but paper has no

colour. Text will have to be changed.

last para before Sec. 4. Cocks et al. here but ref is Kocks. Which

spelling is correct?

Ref 36 needs place of Symposium

Colour is mentioned in captions for Figs 8, 9, and 10. Either the text will

have to be changed or these should be in colour